Paper type: Research paper Pages: 11 (2517 words)
A Study on Use of PlasticWastes for Road ConstructionPragya Sharma1, Manish Kesharwani 2M. Tech. Scholar, Career Point University, Kota1Assistant Professor, Department of Civil Engineering, Career Point University, Kota2*Corresponding AuthorPragya SharmaM.Tech. Scholar, Career Point University, Kota-325003E-mail: [email protected] Mob. No.: 9783215981ABSTRACT: Nowadays, disposal of waste plastic has become a major waste management problem in the world. Plastic is a non-biodegradable material and it is found that the material can remain on earth for 4500 years without degradation. Plastic waste is used as modifier of bitumen to improve some of bitumen properties of Roads that are constructed using plastic waste are known as Plastic Roads and are found to perform better compared to those constructed with conventional bitumen.
Use of higher percentage of plastic waste reduces the need of bitumen by 10%. Hence in this present investigation efforts have made to identify the potential application of waste plastic in civil engineering projects. In this present study the aim is to investigate the optimal use of waste plastic in bitumen for road pavement construction.
From the above experimental investigation it is found that the Stability of 80/100 bitumen at 8% of waste plastic coated on aggregates has shown higher value than that of the 60/70 grade bitumen.KEYWORDS: Bitumen, High Density Polyethylene (HDPE), Low density Polyethylene (LDPE), Marshall Stability method, Waste plastic, Aggregate, Bitumen, plastic-bitumen-aggregate mix, plastic modified bitumen and plastic modified aggregate.INTRODUCTIONNowadays, plastic is everywhere in today’s lifestyle. The term Plastics includes materials composed of various elements such as carbon, hydrogen and oxygen. Plastics are macromolecules, formed by polymerization and having the ability to be shaped by application of reasonable amount of heat and pressure or another form of forces . Plastic is a very versatile material and is found to be almost 5% in municipal solid waste. The experimental studies at several institutes found that the waste plastic, when added to hot aggregate will form a fine coat of plastic over the aggregate and such aggregate, when mixed with the binder is found (a) to give higher strength, (b) higher resistance to water and (c) better performance over a period of time. Plastic waste replaces 10% to 15% of bitumen, and thereby saves approximately Rs.35000 to Rs.45000 per kilometer of a road stretch. Plastic waste in road construction eliminates the plastic shrinkage, cracking of road surface and reduces the drying shrinkage to some extent. The threat of disposal of plastic will not solve until the practical steps are not initiated at the ground level. The field tests withstood the stress and proved that plastic wastes used after proper processing as an additive would enhance the life of the roads and also solve environmental problems. The use of these materials in road making is based on technical, economic, and ecological criteria.Thus, use of waste plastic for the construction is efficient where there is lack of funding and facility is available. II. EXPERIMENTAL INVESTIGATIONObjective The main objective of this experimental investigation is to formulate few testing approach for the evaluation of strength offered by plastic waste mixes. Keeping in view of the above point the following specific objectives have been set for study. Laboratory studies will be carried out on polymer modified asphalt mixtures to evaluate engineering properties using marshal stability. To study basic properties of aggregates and plain bitumen. To study the strength and stability characters of BC (Bitumen Concrete) mix for 60/70 and 80/100 grade bitumen. To study the effect of waste plastic on strength and stability characteristics of BC mix.Cost efficient pavement material.To check the coating property of aggregate with waste plastic materialsMaking environment less harm from plastic wasteExperimental ProgramMaterials UsedThe basic materials for Bitumen Concrete are required such asBitumen,Aggregates,Filler,Waste Plastics.BitumenBitumen is a material which is a byproduct of petroleum refining process. It is a highly viscous at temperatureabove 100 degrees Celsius and is solid at room temperature. For the present investigation 60/70 and 80/100 is employed. Bituminous materials or asphalts are extensively used for roadway construction, primarily because of their excellent binding characteristics and water prolongs properties and relatively low cost. Bituminous materials consists of bitumen which is a black or dark colored solid or viscous cementations substances consists high molecular weight hydrocarbons derived from distillation of petroleum or natural asphalt, has adhesive properties, and is soluble in carbon disulphide . Tars are residues from the destructive distillation of organic substances such as coal, wood, or petroleum and are temperature sensitive than bitumen. Bitumen will be dissolved in petroleum oils where unlike tar doesn’t.Table 1: Properties of bitumen used in present studySr. No. Properties Grades Test Methods60/70 80/100 1. Penetration Tests @27єC 67 90 IS: 1203-19782. Softening Point(R & B)єC 51 41 IS: 1205-19783. Ductility @ 27єC, cm 73.5 75.5 IS: 1208-19794. Specific Gravity of Bitumen 1.017 1.02 IS: 1202-1980AggregatesThe aggregates shall comply to IRC:111-2009, for dense graded mixes and IRC:14-2004, IRC:SP:78-2008 and IRC:11 0-2005 for open graded mixes respectively. Aggregates are tested for strength, toughness, hardness, shape, and water absorption.Table 2: Properties of Aggregates used in present studySr. No. Aggregate tests Test Results Obtained Requirements a per Table 500”4 of MoRT&H (IV Revision) Specifications1. Crushing Value (%) 24.8 -2. Impact Value (%) 20.8 Max. 24%3. Los Angeles Abrasion Value (%) 32 Max. 30%4. Combined Index (%) 29 Max. 30%5. Water Absorption (%) 0.25 Max. 2%6. Specific gravity of coarse Aggregates 2.72 2.5-3.07. Specific gravity of Fine Aggregates 2.76 8. Specific gravity of Filler 2.5 FillerThe filler for dense graded mixes shall comply with IRC:111-2009.PlasticsThe waste plastics are collected from many sources like industries, commercial sector, agricultural sector, andMunicipal sector . After the cleaning of plastic, the waste plastic shall conform to the size passing 2.36 mm sieve and retained on 600-micron sieve. To ascertain the ability of plastic to mix with the binder, the melt-flow value shall be tested as per ASTM D 1238-2010, for which the range shall be as follows:For LDPE: 0.14-58 gm /10 minFor HDPE: 0.02-9.0 gm /10 minAdequate road aggregate have been used and different types of plastics have been used as specified below with the desirable properties as researched by [TCE,2006].Polyethylene Terapthalate (PET) is the type of plastic labeled with the #1 code on or near the bottom of bottles and containers and is commonly used to package soft drinks, water etc. Waste bottle plastic of water cans is made up of either High Density Polyethylene (HDPE) or Low Density Polyethylene (LDPE).Table 3: Properties of plastic used in present studyProperties Results ObtainedSpecific Gravity 1.03Melting Point (єC) 250-260Sieve Analysis Passing 4.75 mm sieve retained on 2.36 mmsieveIII. RESULTS AND DISCUSSIONMarshal test moulds were prepared for different percentages of plain bitumen by varying the bitumen percentage from 3.5% ” 6.5% by increment of 0.5%. The specimens were kept for 24hrs and then were de molded. Marshall Stability test was conducted and parameters like flow value, bulk density, percentage air voids, voids filled with bitumen (VFB) and voids filled with mineral aggregates (VMA) were calculated. The optimum bitumen content,maximum bulk density and 4% volume of voids for bitumen grade 60/70 and 80/100 were calculated using the above properties. Also maximum stability was evaluated. Marshall Stability method was also conducted by adding waste bottle plastic of varying percentage from 0-10% for the know binder content of 60/70 and 80/100 grade bitumen. The maximum stability attained for a particular percentage of plastic is noted down..Table 4: Properties of bituminous mix after adding waste plastic for 60/70 grade bitumenWaste Plastic % GtGb VvVMA VFB VbStability Value, kg Flow Value in 0.25mm0 2.58 2.284 7.701 19.477 60.462 11.776 1231 5.72 2.57 2.285 7.563 19.326 60.865 11.763 1272 64 2.54 2.278 5.343 17.201 68.937 11.858 1291 66 2.52 2.356 5.558 17.273 67.823 11.715 1300 68 2.48 2.284 4.067 15.786 74.238 11.719 1552 610 2.46 2.327 3.776 15.446 75.549 11.668 1525 612 2.43 2.320 2.658 14.283 81.387 11.624 1558 5.7Table 5: Properties of bituminous mix after adding waste plastic for 80/100 grade bitumenWaste Plastic % GtGb VvVMA VFB VbStability Value, kg Flow Value in 0.25mm0 2.60 2.333 11.978 23.612 49.269 11.633 1529 52 2.56 2.330 9.139 20.892 56.255 11.753 1508 54 2.53 2.344 7.636 19.436 60.711 11.800 1609 4.76 2.51 2.325 6.492 18.295 64.518 11.803 1672 4.38 2.49 2.394 4.652 16.580 71.942 11.928 1963 4.710 2.46 2.326 5.842 17.505 66.627 11.663 1736 4.712 2.40 2.315 2.140 13.925 84.631 11.785 1573 4.3lefttop0 Fig.1 For 60/70 grade Bitumen Fig.2 For 80/100 grade Bitumenlefttop0 Fig.3 For 60/70 grade Bitumen Fig.4 For 80/100 grade Bitumenlefttop Fig.5 For 60/70 grade Bitumen Fig.6 For 80/100 grade Bitumenlefttop00 Fig.7 For 60/70 grade Bitumen Fig.8 For 80/100 grade Bitumenlefttop Fig.9 For 60/70 grade Bitumen Fig.10 For 80/100 grade BitumenFig.11 Comparison of stability values of 60/70 and 80/100 IV. DISCUSSIONSFrom the above investigation it is observed that Optimum bitumen content obtained for bituminous concrete grade I mix for 60/70 grade bitumen was 5% and 80/100 grade bitumen was 5.1% as per the specification of MORT&H standards. The stability obtained for the respective OBC was 12.606 Kn and 17.334 Kn. Waste shredded plastic bottle were added in the increasing percentage of 0% – 12% to bituminous concrete mix and an Addition of 2% to 12% waste shredded plastic bottles by the weight of bitumen to BC mix has resulted in following: Stability of 80/100 bitumen at 8% of waste plastic coated on aggregates has shown higher value than that of the 60/70 grade bitumen. The stability value of the mix in unsoaked condition has high values than compared to the soaked specimens. Stability value decreases as the soaking time of the specimen increases. Specimen with 3days soaking results in least stability than that of 1day and 2day soaking periods.FOR PLAIN 60/70 BITUMENa) The waste plastic which is added to aggregate mix by heating upto 260-2800C. then the bitumenis added to form the grade I bituminous concrete and optimum bitumen content of 5% has shownthe following results: The maximum stability was 1552 Kg at 8% waste plastic by the weight of bitumen, 6mm flow at 8% waste plastic and 74.238 VFB at 8% waste plasticBulk density “b was found to be maximum of2.356 gm/cc at 6% waste plastic and then reduces to 2.284 gm/cc at 8% waste plastic. Voids in the total mix Vv varies from 4% to 10% by varying the waste plastic content from 2% – 12% and at 8% waste plastic Vv was found to be 4.067%.b) By blending shredded waste plastic to the bitumen by heating and then adding the required aggregate to form BC mix grade I resulted in improper mix and stability obtained is less than that of the optimum binder content [OBC]. This is due to following: Improper blending of plastic in bitumen. This is because the melting point of poly ethylene teraphthalate [PET] is 260-2800єC Since the melting temperature of plastic is too high it is difficult to melt plastic in bitumen to get a proper blend. Bitumen should be heated up to the temperature of 260-2800C in order to obtain the proper blend. If this is done there will be a chance of bitumen to catch fire and also there will be a loss in weight of bitumen.FOR PLAIN 80/100 BITUMENa) The waste plastic which is added to aggregate mix by heating upto 260-2800C. Then the bitumen is added to form the grade I bituminous concrete and optimum bitumen content of 5% has shown the following results: The maximum stability was 1963 Kg at 8% waste plastic by the weight of bitumen, 4.7mm flow at 8% waste plastic and 71.942 VFB at 8% waste plastic Bulk density “b was found to be maximum of 2.394 gm/cc at 8% waste plastic and then reduces to 2.315 gm/cc at 12% waste plastic. Voids in the total mix Vv varies from 8% to 10% by varying the waste plastic content from 2% – 12% and at 8% waste plastic Vv was found to be 4.652%.b) By blending shredded waste plastic to the bitumen by heating and then adding the required aggregate to form BC mix grade I resulted in improper mix and stability obtained is less than that of the optimum binder content [OBC]. This is due to following: Improper blending of plastic in bitumen. This is because the melting point of poly ethylene teraphthalate [PET] is 260-2800єC. Since the melting temperature of plastic is too high it is difficult to melt plastic in bitumen to get a proper blend.Bitumen should be heated up to the temperature of 260-2800C in order to obtain the proper blend. If this is done there will be a chance of bitumen to catch fire and also there will be a loss in weight of bitumen. All the parameters like stability, flow, bulk density, voids and VFB shows that, the addition of waste plastic in mix has no much change in fluidity and rigidity parameters as compared to that of plain bituminous mix.V. CONCLUSIONIn the present study, the importance was to add the shredded waste plastic bottles to bituminousconcrete (BC) mix and to evaluate the various mix properties like Marshall Stability, flow, bulkdensity, voids in the mix and VFB. Also the effect of soaking conditions of the mix was investigated.Indirect tensile strength was investigated for OBC and 8% plastic coated on aggregates which had yielded the highest marshal stability.The optimum plastic content for 60/70 and 80/100 grade bitumen was 8%.For both 60/70 and 80/100 grade bitumen with plastic content 8%, the maximum stability was achieved in 80/100 grade bitumen.Wet process i.e. blending of plastic and bitumen cannot be carried out due to the plastic which is used has a very high melting point.There is an increase in stability up to 15% and 10% after adding waste plastic to the mix in 60/70 and 80/100 grade bitumen respectively. There is a decrease in stability value in water sensitivity test results. Unsoaked specimens show high stability value but soaked specimens showed a decreasing stability value. Hence there is an increase in stability with the addition of PET plastic in asphalt mix by incorporating dry process this can be used in highway construction for better stability for the appropriate trafficREFERENCES1. Mahabir Panda and Mayajit Mazumdar(1999). Engineering Properties of EVA-Modified Bitumen For Paving Mixes. Journal Of Materials In Civil EngineeringASCE / May 19992. Romona, Ledesma and Isacc8 L. L. Effect of Poly Ethylene Teraphthalate from Plastic Waste on the Thermal Properties of Asphalt. The City College of Cuny Dept.of Chemical Engineering New York.3. Punith V.S and Veeraraghavan A (2007). Behavior of Asphalt Concrete Mixtures with Reclaimed Polyethylene as Additive. Journal Of Materials In CivilEngineering ASCE / June 2007 / 5014. Sabina, Tabrez A Khan, Sangita, Sharma D K and Sharma B M (2009). Performance Evaluation Of Waste Plastic/Polymer Modified Bituminous Concrete Mixes.Journal of scientific and industrial research Vol.68, November 2009, pp. 975-979.5. Khanna S K, Justo C E G and Veeraragavan A (2000). Highway Material And Pavement Testing (Laboratory Manual), Nemchand and Bros, Roorkee 2000.6. Ministry of Road Transport and Highways (2001). Specifications for road and bridge works Fourth Revision, Published by Indian Road Congress on behalf of theGovernment of India.7. Global Plastic Production Rises, Recycling Lags- New Worldwatch Institute analysis explores trends in global plastic consumption and recycling-8. IS: 383-1970 and IS: 2386(1963).9. test/10.
Cite this page
Research Paper. (2019, Aug 20). Retrieved from https://studymoose.com/research-paper-10-essay